The strong correlations between thermal conductivities and electronic spin states in crystals of Fe(III) spin crossover complexes
Hoshino, Norihisa; Hayashi, Akari; Akutagawa, Tomoyuki; Dalton Transactions  (2022) –; doi:10.1039/D2DT01597H

data_7710848
_publ_section_title
;
 The strong correlations between thermal conductivities and electronic
 spin states in crystals of Fe(III) spin crossover complexes
;
_journal_name_full               'Dalton Transactions'
_journal_paper_doi               10.1039/D2DT01597H
_journal_year                    2022
_chemical_formula_moiety         'C22 H28 Br2 Fe N4 O2 1+, C F3 O3 S 1-'
_chemical_formula_sum            'C23 H28 Br2 F3 Fe N4 O5 S'
_chemical_formula_weight         745.22
_space_group_crystal_system      monoclinic
_space_group_IT_number           14
_space_group_name_Hall           '-P 2ybc'
_space_group_name_H-M_alt        'P 1 21/c 1'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     dual
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-2018/3
_audit_update_record
;
2022-07-07 deposited with the CCDC.	2022-07-28 downloaded from the CCDC.
;
_cell_angle_alpha                90
_cell_angle_beta                 107.220(8)
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   9.4977(16)
_cell_length_b                   24.352(4)
_cell_length_c                   12.701(2)
_cell_measurement_reflns_used    2976
_cell_measurement_temperature    232(2)
_cell_measurement_theta_max      68.28
_cell_measurement_theta_min      3.63
_cell_volume                     2805.9(8)
_computing_cell_refinement       'RAPID AUTO (Rigaku, 2011)'
_computing_data_collection       'RAPID AUTO (Rigaku, 2011)'
_computing_data_reduction        'RAPID AUTO (Rigaku, 2011)'
_computing_molecular_graphics    'Mercury (CCDC, 2020)'
_computing_publication_material  'SHELXL-2018/3 (Sheldrick, 2018)'
_computing_structure_refinement  'SHELXL-2018/3 (Sheldrick, 2018)'
_computing_structure_solution    'SHELXT 2018/2 (Sheldrick, 2018)'
_diffrn_ambient_temperature      232(2)
_diffrn_detector_area_resol_mean 10.000
_diffrn_measured_fraction_theta_full 0.988
_diffrn_measured_fraction_theta_max 0.987
_diffrn_measurement_device_type  'Rigaku R-AXIS RAPID'
_diffrn_measurement_method       \w
_diffrn_radiation_type           CuK\a
_diffrn_radiation_wavelength     1.54187
_diffrn_reflns_av_R_equivalents  0.1187
_diffrn_reflns_av_unetI/netI     0.0905
_diffrn_reflns_Laue_measured_fraction_full 0.988
_diffrn_reflns_Laue_measured_fraction_max 0.987
_diffrn_reflns_limit_h_max       11
_diffrn_reflns_limit_h_min       -10
_diffrn_reflns_limit_k_max       28
_diffrn_reflns_limit_k_min       -29
_diffrn_reflns_limit_l_max       15
_diffrn_reflns_limit_l_min       -14
_diffrn_reflns_number            30418
_diffrn_reflns_point_group_measured_fraction_full 0.988
_diffrn_reflns_point_group_measured_fraction_max 0.987
_diffrn_reflns_theta_full        67.687
_diffrn_reflns_theta_max         68.243
_diffrn_reflns_theta_min         3.630
_diffrn_source                   'rotating-anode X-ray tube'
_exptl_absorpt_coefficient_mu    8.891
_exptl_absorpt_correction_T_max  0.9973
_exptl_absorpt_correction_T_min  0.3444
_exptl_absorpt_correction_type   empirical
_exptl_absorpt_process_details   'ABSCOR (Rigaku, 2011)'
_exptl_crystal_colour            black
_exptl_crystal_density_diffrn    1.764
_exptl_crystal_description       block
_exptl_crystal_F_000             1492
_exptl_crystal_preparation       'Magnetic properties,Thermal conductivity'
_exptl_crystal_size_max          0.100
_exptl_crystal_size_mid          0.100
_exptl_crystal_size_min          0.100
_refine_diff_density_max         0.605
_refine_diff_density_min         -1.524
_refine_diff_density_rms         0.160
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.156
_refine_ls_hydrogen_treatment    constr
_refine_ls_matrix_type           full
_refine_ls_number_parameters     352
_refine_ls_number_reflns         5086
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.156
_refine_ls_R_factor_all          0.1407
_refine_ls_R_factor_gt           0.0838
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[\s^2^(Fo^2^)+(0.1527P)^2^] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.2144
_refine_ls_wR_factor_ref         0.3006
_reflns_Friedel_coverage         0.000
_reflns_number_gt                2766
_reflns_number_total             5086
_reflns_threshold_expression     'I > 2\s(I)'
_cod_data_source_file            d2dt01597h2.cif
_cod_data_source_block           3_232K
_cod_original_cell_volume        2805.8(8)
_cod_original_sg_symbol_H-M      'P 21/c'
_cod_database_code               7710848
_shelx_shelxl_version_number     2018/3
_shelx_estimated_absorpt_t_min   0.470
_shelx_estimated_absorpt_t_max   0.470
_shelx_res_checksum              18161
_shelx_hkl_checksum              97822